Large-scale synthesis of highly emissive and photostable CuInS2/ZnS nanocrystals through hybrid flow reactor
© Lee and Han; licensee Springer. 2014
Received: 3 January 2014
Accepted: 5 February 2014
Published: 17 February 2014
We report a high-yield, low-cost synthesis route to colloidal CuInS2/ZnS (CIS/ZnS) nanocrystals (NCs) with Cu vacancies in the crystal lattice. Yellow-emitting CIS/ZnS core/shell NCs of high luminescence were facilely synthesized via a stepwise, consecutive hybrid flow reactor approach. It is based on serial combination of a batch-type mixer and a flow-type furnace. In this reactor, the flow rate of the solutions was typically 1 mL/min, 100 times larger than that of conventional microfluidic reactors. This method can produce gram quantities of material with a chemical yield in excess of 90% with minimal solvent waste. This is a noninjection-based approach in 1-dodecanethiol (DDT) with excellent synthetic reproducibility and large-scale capability. The optical features and structure of the obtained CIS/ZnS NCs have been characterized by UV–vis and fluorescence spectroscopies, X-ray diffraction (XRD), X-ray photoelectron spectroscopy (XPS), energy-dispersive X-ray spectroscopy (EDX) and high-resolution transmission electron microscopy (HRTEM). The resulting CIS/ZnS NCs in chloroform exhibit quantum yield (QY) of 61.4% with photoemission peaking at 561 nm and full width at half maximum (FWHM) of 92 nm. The as-synthesized CIS/ZnS NCs were proven to have excellent photostability. The synthesized CIS/ZnS NCs can be a promising fluorescent probe for biological imaging and color converting material for light-emitting diode due to Cd-free constituents.
KeywordsCuInS2/ZnS nanocrystals Hybrid flow reactor Large-scale synthesis Photostability
Semiconductor nanocrystals (NCs, or quantum dots, QDs) have attracted enormous interests in the last decade as a novel class of material due to their special properties and a wide area of potential applications[1–3], such as biomedical labeling, light-emitting diodes (LEDs), solar cells, lasers, and sensors[4–9]. Among them, cadmium-contained NCs, including CdSe, CdS, and CdTe, have been major research topics due to their good electrical and optical properties, but the inherent toxicity of cadmium limits their applications especially in the biomedical and industrial areas. Commercial products must meet safety standards and comply with regulations. It is partly for this reason, NCs synthesized from the III-V group elements (InP) and from the I-III-VI2 group (CuInS2 and CuInSe2) attracted most interest and lately have reached the performance level comparable to their Cd-based equivalents. These are attractive alternatives to Cd-based QDs due to their nontoxic behavior[10–16].
Among these, CuInS2 (CIS) NCs with a bulk band gap of 1.5 eV (827 nm) is selected as an important candidate for optical application and their high potential in solar energy conversion[18–32]. CIS NCs are of particular interest in photovoltaic applications for its high energy conversion efficiency, high absorption coefficient, radiation stability, and low toxicity. Theoretical calculations indicate that the Wannier-Mott bulk exciton radius of CIS NCs is 4.1 nm. It was expected that the CIS NCs with size comparable to Wannier-Mott bulk exciton radius are suitable materials for nanocrystal solar cells and nontoxic luminescent compounds. Thus, it is of very importance to synthesize the CIS NCs with their size smaller than 10 nm. So far, CIS has motivated the development of many synthetic approaches including a solvothermal method[18–21], a precursor decomposition method (thermolysis)[22, 23, 31], photochemical decomposition, and hot injection techniques[25–30, 32].
Recently, several works on the synthesis of CIS NCs and an efficient route to highly luminescent CIS/ZnS core-shell NCs were reported[9, 33–35]. To improve their photoluminescence (PL) emission properties, shell coating and alloying strategies have been adapted to produce high quality CIS NCs[36–48]. Literature reports have revealed that stoichiometry control is very important in the production of highly luminescent CIS NCs[23, 36–48]. In addition, CIS NCs have the characteristic of long PL lifetime, which was thought to be related to intrinsic defects. Based on theoretical models and experimental works on bulk materials, the intrinsic defects of CIS materials have been found to be related to off-stoichiometry effects[46, 47]. Although stoichiometry control of CIS NCs has been reported, it is still of great interest to further understand off-stoichiometry effects on the physical properties of CIS NCs[49, 50].
In the present study, a facile, stepwise hybrid flow reactor method is demonstrated for the first time to synthesize highly fluorescent CIS/ZnS NCs. This reactor is formed based on consecutive combination of the batched mixer and the tube furnace with flowing solution. The flow rate of this reactor was ca. 100 times larger than common microfluidics reactors. In order to synthesize high quality CIS/ZnS NCs, we adjusted the concentrations of reactants and the growing temperature. First, CIS core NCs were thermally grown at 210°C for reaction times of 1 min and then ZnS shell overcoating was consecutively conducted via the thermolysis method (320°C for 2 min). The resulting NCs were subsequently overcoated with a ZnS shell using a mixture of zinc acetate, oleic acid, 1-dodecanethiol, and trioctylamine. During the shell growth, the PL quantum yield (QY) strongly increased to values of 20% to 60%. The resulting CIS/ZnS NCs exhibited emissions of yellow with a maximum quantum yield of 61.4%. Both band gap and peak emission energies of CIS/ZnS core/shell NCs were substantially blueshifted compared to that of the original CIS core counterparts (red emission). We provide a simple and reliable synthesis method for CIS-based NCs showing increased fluorescence QY and high photostability.
Cu(I) iodide (CuI, Aldrich, Yongin City, Kyunggi-do, South Korea, 98%), In acetate (In(OAc)3, Aldrich, 99.99%), 1-dodecanethiol (DDT, Aldrich, 98%), 1-octadecene (ODE, Aldrich, 90%), Zn acetate (Zn(OAc)2, Aldrich, 99.99%), trioctylamine (TOA, Aldrich, 98%), and oleic acid (OA, Alfa Aesar, 90%) were used without further purification.
Synthesis of CIS core
In a typical synthetic procedure of CIS NCs with [Cu]/[In] molar ratios of 0.5, CuI (0.0476 g, 0.25 mmol) and In(OAc)3 (0.1460 g, 0.5 mmol) were mixed with DDT (5 mL) in a 100 mL two-necked flask, which was followed by the addition of ODE (4 mL). The reaction mixture was degassed under vacuum for 10 min at 150°C. Next, the solution was heated to 210°C for 1 min under nitrogen flow until a deep red colloidal solution was formed. Afterward, the reaction solution was cooled to room temperature.
Synthesis of ZnS overcoating
To make the Zn and S precursor mixture in flask, 1.46 g of zinc acetate was dissolved in 8 mL of TOA with 4 mL of OA, then mixed with 4 mL of DDT. The resulting mixture was stirred at 100°C for several minutes under vacuum. After cooling down to room temperature, a pump carried the solution (CIS cores plus Zn and S precursors) to furnace (320°C), where ZnS shells were grown on the CIS cores. Finally, the resultant CIS/ZnS core/shell NCs solution was collected at the exit of furnace.
Purification of CIS/ZnS NCs
The NC dispersions were diluted by the addition of chloroform. The solutions were precipitated with an excess of methanol and 1-butanol. The flocculent precipitate was centrifuged at 4,000 rpm for 2 min and the supernatant decanted. This process was repeated a minimum of three times, and the precipitation was then dried to powder for characterization.
Optical characterization of the CIS/ZnS NCs was carried out using a UV–vis spectrophotometer (Optizen 2120, Mecasys, Korea), a fluorometer (Fluorolog, Horiba Jobin Yvon, France), and an absolute QY measurement system (C-9920-02, Hamamatsu, Japan). X-ray diffraction analysis was performed using a D/MAX Ultima III diffractometer (Rigaku Corporation, Tokyo, Japan) operated at a 40 kV voltage and a 40 mA current with Cu Kα radiation. Data were collected at room temperature in the 5° to 80° range at increments of 0.02°. High-resolution transmission electron microscopy (HRTEM) observations were obtained using a Tecnai G2 F30 S-Twin model (FEI, Hillsboro, OR, USA) at 300 kV. To conduct an investigation by TEM, the NCs were deposited from dilute chloroform solutions onto copper grids with carbon support by slowly evaporating the solvent in air at room temperature. Energy-dispersive X-ray spectroscopy (EDX) analyses of samples were carried out with a Hitachi S-4700 (Hitachi Ltd., Chiyoda-ku, Japan) scanning electron microscopy equipped with an energy-dispersive X-ray analyzer. The photoelectron spectra were obtained with a ESCA-2000 Multilab apparatus (VG Microtech, East Grinstead, West Sussex, UK) using a nonmonochromatic Mg Kα excitation source and a hemispherical analyzer. The residual gas pressure in the chamber during the measurements was approximately 10−10 Torr. All spectra were recorded at 90° takeoff angle with a pass energy of 20 eV and at an instrumental resolution of 0.9 eV. The stability of the CIS/ZnS NCs against photooxidation was assessed by placing them into quartz cuvettes with half of the volume being filled with air and continuously irradiating them with a UV lamp (365 nm, distance lamp sample, 10 cm). The photodegradation was monitored by taking PL spectra at certain time intervals.
Results and discussion
In summary, highly luminescent CIS/ZnS core/shell NCs with a quantum yield of 61.4% were synthesized on a large scale using a hybrid flow reactor in a simple, one-step process. XRD, XPS, EDX, and HRTEM characterizations show that the fabricated CIS/ZnS NCs are of high quality. This newly developed synthetic methodology is ideal in a number of ways as it can be easily altered to yield a high-quality product on a gram scale with low loss, is highly reproducible, and is based on green chemistry. In the present work, the photostability of high-quality CIS/ZnS NCs was investigated at ambient condition both under UV irradiation and in the darkness. The as-synthesized CIS/ZnS NCs were proven to have excellent photostability. In addition, this method can also be simply extended to AgInS2, Zn x (CuIn)1-xS2 and CuGa x In1-xS2 systems, which are also of interest for light emitting, biolabel, and solar harvesting applications.
This work was supported by the Industrial Strategic technology development program (no. 10035274, ‘Quantum dot phosphorus converted LED module’) funded by the Ministry of Trade, Industry and Energy (MOTIE), Korea.
- Yong K: Quantum dots for biophotonics. Theranostics 2012, 2: 629–630. 10.7150/thno.4757View Article
- Yong K, Wang Y, Roy I, Rui H, Swihart MT, Law W, Kwak SK, Ye L, Liu J, Mahajan SD, Reynolds JL: Preparation of quantum dot/drug nanoparticle formulations for traceable targeted delivery and therapy. Theranostics 2012, 2: 681–694. 10.7150/thno.3692View Article
- Guo W, Chen N, Tu Y, Dong C, Zhang B, Hu C, Chang J: Synthesis of Zn-Cu-In-S/ZnS core/shell quantum dots with inhibited blue-shift photoluminescence and applications for tumor targeted bioimaging. Theranostics 2013, 3: 99–108. 10.7150/thno.5361View Article
- Bruchez JM, Moronne M, Gin P, Weiss S, Alivisatos AP: Semiconductor nanocrystals as fluorescent biological labels. Science 1998, 281: 2013–2016.View Article
- Murray CB, Kagan CR, Bawendi MG: Synthesis and characterization of monodisperse nanocrystals and close-packed nanocrystal assembles. Annu Rev Mater Sci 2000, 30: 545–610. 10.1146/annurev.matsci.30.1.545View Article
- Chan WCW, Nie S: Quantum dot bioconjugates for ultrasensitive nonisotopic detection. Science 1998, 281: 2016–2018.View Article
- Colvin VL, Schlamp MC, Alivisatos AP: Light-emitting diodes made from cadmium selenide nanocrystals and a semiconducting polymer. Nature 1994, 370: 354–357. 10.1038/370354a0View Article
- Klimov VI, Mikhailovsky AA, Xu S, Malko A, Hollingsworth JA, Leatherdale CA, Eisler HJ, Bawendi MG: Optical gain and stimulated emission in nanocrystal quantum dots. Science 2000, 290: 314–317. 10.1126/science.290.5490.314View Article
- Li L, Daou TJ, Texier I, Chi TTK, Liem NQ, Reiss P: Highly luminescent CuInS2/ZnS core/shell nanocrystals: cadmium-free quantum dots for in vivo imaging. Chem Mater 2009, 21: 2422–2429. 10.1021/cm900103bView Article
- Kim S, Kim T, Kang M, Kwak SK, Yoo TW, Park LS, Yang I, Hwang S, Lee JE, Kim SK, Kim S: Highly luminescent InP/GaP/ZnS nanocrystals and their application to white light-emitting diodes. J Am Chem Soc 2012, 134: 3804–3809. 10.1021/ja210211zView Article
- Song W, Yang H: Efficient white-light-emitting diodes fabricated from highly fluorescent copper indium sulfide core/shell quantum dots. Chem Mater 2012, 24: 1961–1967. 10.1021/cm300837zView Article
- Song W, Yang H: Fabrication of white light-emitting diodes based on solvothermally synthesized copper indium sulfide quantum dots as color converters. Appl Phys Lett 2012, 100: 1831041–1831043.
- Tan Z, Zhang Y, Xie C, Su H, Liu J, Zhang C, Dellas N, Mohoney SE, Wang Y, Wang J, Xu J: Near-band-edge electroluminescence from heavy-metal-free colloidal quantum dots. J Adv Mater 2011, 23: 3553–3558. 10.1002/adma.201100719View Article
- Wood V, Halpert JE, Panzer MJ, Bawendi MG, Bulovič V: Alternating current driven electroluminescence from ZnSe/ZnS:Mn/ZnS nanocrystals. Nano Lett 2009, 9: 2367–2371. 10.1021/nl900898tView Article
- Menkara H, Gilstrap JRA, Morris T, Minkara M, Wagner BK, Summers CJ: Development of nanophosphors for light emitting diodes. Opt Express 2011, 19: A972-A981. 10.1364/OE.19.00A972View Article
- Anc MJ, Pickett NL, Gresty NC, Harris JA, Mishra KC: Progress in non-Cd quantum dot development for lighting applications. ECS Journal of Solid State Science and Technology 2013, 2: R3071-R3082.View Article
- Jaffe JE, Zunger A: Theory of the band-gap anomaly in ABC2 chalcopyrite semiconductors. Phys Rev B 1984, 29: 1882–1906. 10.1103/PhysRevB.29.1882View Article
- Xiao J, Xie Y, Xiong Y, Tang R, Qian YT: A mild solvothermal route to chalcopyrite quaternary semiconductor CuIn(SexS1-x)2 nanocrystallites. J Mater Chem 2001, 11: 1417–1420. 10.1039/b100092fView Article
- Li B, Xie Y, Huang J, Qian YT: Synthesis by a solvothermal route and characterization of CuInSe2 nanowhiskers and nanoparticles. Adv Mater 1999, 11: 1456–1459. 10.1002/(SICI)1521-4095(199912)11:17<1456::AID-ADMA1456>3.0.CO;2-3View Article
- Jiang Y, Wu Y, Mo X, Yu WC, Xie Y, Qian YT: Elemental solvothermal reaction to produce ternary semiconductor CuInE2 (E = S, Se) nanorods. Inorg Chem 2000, 39: 2964–2965. 10.1021/ic000126xView Article
- Gou X, Cheng F, Shi Y, Zhang L, Peng S, Chen J, Shen P: Shape-controlled synthesis of ternary chalcogenide ZnIn2S4 and CuIn(S, Se)2 nano-/microstructures via facile solution route. J Am Chem Soc 2006, 128: 7222–7229. 10.1021/ja0580845View Article
- Castro SL, Bailey SG, Raffaelle RP, Banger KK, Hepp AF: Nanocrystalline chalcopyrite materials (CuInS2 and CuInSe2) via low-temperature pyrolysis of molecular single-source precursors. Chem Mater 2003, 15: 3142–3147. 10.1021/cm034161oView Article
- Zhong H, Zhou Y, Ye M, He Y, Ye J, He C, Yang C, Li Y: Controlled synthesis and optical properties of colloidal ternary chalcogenide CuInS2 nanocrystals. Chem Mater 2008, 20: 6434–6443. 10.1021/cm8006827View Article
- Nairn JJ, Shapiro PJ, Twamley B, Pounds T, Von Wandruszka R, Fletcher TR, Williams M, Wang C, Norton MG: Preparation of ultrafine chalcopyrite nanoparticles via the photochemical decomposition of molecular single-source precursors. Nano Lett 2006, 6: 1218–1223. 10.1021/nl060661fView Article
- Malik MA, O’Brien P, Revaprasadu N: A novel route for the preparation of CuSe and CuInSe2 nanoparticles. Adv Mater 1999, 11: 1441–1444. 10.1002/(SICI)1521-4095(199912)11:17<1441::AID-ADMA1441>3.0.CO;2-ZView Article
- Zhong H, Li Y, Ye M, Zhu Z, Zhou Y, Yang C, Li Y: A facile route to synthesize chalcopyrite CuInSe2 nanocrystals in non-coordinating solvent. Nanotechnology 2007, 18(025602):6.
- Pan DC, An LJ, Sun ZM, Hou W, Yang Y, Yang ZZ, Lu YF: Synthesis of Cu-In-S ternary nanocrystals with tunable structure and composition. J Am Chem Soc 2008, 130: 5620–5621. 10.1021/ja711027jView Article
- Guo QJ, Kim SJ, Kar M, Shafarman WN, Birkmire RW, Stach EA, Agrawal R, Hillhouse HW: Development of CuInSe2 nanocrystal and nanoring inks for low-cost solar cells. Nano Lett 2008, 8: 2982–2987. 10.1021/nl802042gView Article
- Banger KK, Jin MHC, Harris JD, Fanwick PE, Hepp AF: A new facile route for the preparation of single-source precursors for bulk, thin-film, and nanocrystallite I-III-VI semiconductors. Inorg Chem 2003, 42: 7713–7715. 10.1021/ic034802hView Article
- Arici E, Sariciftci NS, Meissner D: Hybrid solar cells based on nanoparticles of CuInS2 in organic matrices. Adv Funct Mater 2003, 13: 165–171. 10.1002/adfm.200390024View Article
- Panthani MG, Akhavan V, Goodfellow B, Schmidtke JP, Dunn L, Dodabalapur A, Barbara PF, Korgel BA: Synthesis of CuInS2, CuInSe2, and Cu(In x Ga1-x)Se2 (CIGS) nanocrystal “inks” for printable photovoltaics. J Am Chem Soc 2008, 130: 16770–16777. 10.1021/ja805845qView Article
- Tang J, Hinds S, Kelley SO, Sargent EH: Synthesis of colloidal CuGaSe2, CuInSe2, and Cu(InGa)Se2 nanoparticles. Chem Mater 2008, 20: 6906–6910. 10.1021/cm801655wView Article
- Nose K, Soma Y, Omata T, Otsuka-Yao-Matsuo S: Synthesis of ternary CuInS2 nanocrystals; phase determination by complex ligand species. Chem Mater 2009, 21: 2607–2613. 10.1021/cm802022pView Article
- Li L, Pandey A, Werder DJ, Khanal BP, Pietryga JM, Klimov VI: Efficient synthesis of highly luminescent copper indium sulfide-based core/shell nanocrystals with surprisingly long-lived emission. J Am Chem Soc 2011, 133: 1176–1179. 10.1021/ja108261hView Article
- Park J, Kim SW: CuInS2/ZnS core/shell quantum dots by cation exchange and their blue-shifted photoluminescence. J Mater Chem 2011, 21: 3745–3750. 10.1039/c0jm03194aView Article
- Zhong HZ, Lo SS, Mirkovic T, Li Y, Ding Y, Li Y, Scholes GD: Noninjection gram-scale synthesis of monodisperse pyramidal CuInS2 nanocrystals and their size-dependent properties. ACS Nano 2010, 4: 5253–5262. 10.1021/nn1015538View Article
- Toromoto T, Ogawa S, Adachi T, Kameyama T, Okazaki K, Shibayama T, Kuno A, Kuwabata S: Remarkable photoluminescence enhancement of ZnS-AgInS2 solid solution nanoparticles by post-synthesis treatment. Chem Commun 2010, 46: 2082–2084. 10.1039/b924186hView Article
- Tang XS, Cheng WL, Choo ESG, Xue JM: Synthesis of CuInS2-ZnS alloyed nanocubes with high luminescence. Chem Commun 2011, 47: 5217–5219. 10.1039/c1cc10417aView Article
- Tang XS, Yu K, Xu Q, Choo ESG, Goh GKL, Xue JM: Synthesis and characterization of AgInS2-ZnS heterodimers with tunable photoluminescence. J Mater Chem 2011, 21: 11239–11243. 10.1039/c1jm11346aView Article
- Zhang WJ, Zhong XH: Facile synthesis of ZnS-CuInS2-alloyed nanocrystals for a color-tunable fluorchrome and photocatalyst. Inorg Chem 2011, 50: 4065–4072. 10.1021/ic102559eView Article
- Feng J, Sun M, Yang F, Yang XR: A facile approach to synthesize high-quality ZnxCuyInS1.5+x+0.5y nanocrystal emitters. Chem Commun 2011, 47: 6422–6424. 10.1039/c1cc11754hView Article
- Zhang J, Xie RG, Yang WS: A simple route for highly luminescent quaternary Cu-Zn-In-S nanocrystal emitters. Chem Mater 2011, 23: 3357–3361. 10.1021/cm201400wView Article
- Zhong HZ, Wang ZB, Bovero E, Lu ZH, Van Veggel FCJM, Scholes GD: Colloidal CuInSe2 nanocrystals in the quantum confinement regime: synthesis, optical properties, and electroluminescence. J Phys Chem C 2011, 115: 12396–12402. 10.1021/jp204249jView Article
- Sarkar S, Karan NS, Pradhan N: Ultrasmall color-tunable copper-doped ternary semiconductor nanocrystal emitters. Angew Chem Int Ed 2011, 50: 6065–6069. 10.1002/anie.201101572View Article
- Hamanaka Y, Kuzuya T, Sofue T, Kino T, Ito K, Sumiyama K: Defect-induced photoluminescence and third-order nonlinear optical response of chemically synthesized chalcopyrite CuInS2 nanoparticles. Chem Phys Lett 2008, 466: 176–180. 10.1016/j.cplett.2008.10.055View Article
- Zhang SB, Wei SH, Zunger A, Katayama-Yoshida H: Defect physics of the CuInSe2 chalcopyrite semiconductor. Phys Rev B 1998, 57: 9642–9656. 10.1103/PhysRevB.57.9642View Article
- Dagan AG, Abou-Elfotouh F, Dunlavy DJ, Matson RJ, Cahen D: Defect level identification in CuInSe2 from photoluminescence studies. Chem Mater 1990, 2: 286–293. 10.1021/cm00009a019View Article
- Uehara M, Watanabe K, Tajiri Y, Nakamura H, Maeda H: Synthesis of CuInS2 fluorescent nanocrystals and enhancement of fluorescence by controlling crystal defect. J Chem Phys 2008, 129: 1347091–1347096.View Article
- Kim Y, Ahn S, Chung K, Cho Y, Choi C: The photoluminescence of CuInS2 nanocrystals: effect of non-stoichiometry and surface modification. J Mater Chem 2012, 22: 1516–1520. 10.1039/c1jm13170bView Article
- Chen B, Zhong H, Zhang W, Tan Z, Li Y, Yu C, Zhai T, Bando Y, Yang S, Zou B: Highly emissive and color-tunable CuInS2-based colloidal semiconductor nanocrystals: off-stoichiometry effects and improved electroluminescence performance. Adv Funct Mater 2012, 22: 2081–2088. 10.1002/adfm.201102496View Article
- Kim K, Jeong S, Woo JY, Han CS: Successive and large-scale synthesis of InP/ZnS quantum dots in a hybrid reactor and their application to white LEDs. Nanotechnology 2012, 23(065602):7.
- Nam DE, Song WS, Yang H: Facile, air-insensitive solvothermal synthesis of emission-tunable CuInS2/ZnS quantum dots with high quantum yields. J Mater Chem 2011, 21: 18220–18226. 10.1039/c1jm12437dView Article
- Talapin DT, Rogach AL, Kornowski A, Haase M, Weller H: Highly luminescent monodisperse CdSe and CdSe/ZnS nanocrystals synthesized in a hexadecylamine-trioctylphosphine oxide-trioctylphospine mixture. Nano Lett 2001, 1: 207–211. 10.1021/nl0155126View Article
- Dabbousi BO, Rodriguez-Viejo J, Mikulec FV, Heine JR, Mattoussi H, Ober R, Jensen KF, Bawendi MG: (CdSe)ZnS core-shell quantum dots: synthesis and characterization of a size series of highly luminescent nanocrystallites. J Phys Chem B 1997, 101: 9463–9475. 10.1021/jp971091yView Article
- Moulder JF, Stickle WF, Sobol PE, Bomben K: Handbook of X-ray photoelectron spectroscopy. Eden Prairie: Perkin-Elmer Corporation, Physical Electronics Division; 1992.
- Yue W, Han S, Peng R, Shen W, Geng H, Wu F, Tao S, Wang M: CuInS2 quantum dots synthesized by a solvothermal route and their application as effective electron acceptors for hybrid solar cells. J Mater Chem 2010, 20: 7570–7578. 10.1039/c0jm00611dView Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.